#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/92/4309215.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4309215
loop_
_publ_author_name
'William H. Casey'
'Marilyn M. Olmstead'
'Brian L. Phillips'
_publ_section_title
;
A New Aluminum Hydroxide Octamer, [Al8(OH)14(H2O)18](SO4)5.16H2O
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4888
_journal_page_last               4890
_journal_paper_doi               10.1021/ic050426k
_journal_volume                  44
_journal_year                    2005
_chemical_formula_moiety         'Al8 H50 O32, 5(S O4), 16(H2 O)'
_chemical_formula_sum            'Al8 H82 O68 S5'
_chemical_formula_weight         1546.80
_chemical_name_common            '[Al8(OH)14(H2O)18](SO4)5.16H2O'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                99.585(6)
_cell_angle_beta                 102.932(6)
_cell_angle_gamma                110.311(6)
_cell_formula_units_Z            1
_cell_length_a                   9.236(3)
_cell_length_b                   11.994(4)
_cell_length_c                   14.694(5)
_cell_measurement_reflns_used    914
_cell_measurement_temperature    90(2)
_cell_measurement_theta_max      30.4
_cell_measurement_theta_min      2.4
_cell_volume                     1433.7(8)
_computing_cell_refinement       'SAINT 7.16B (Bruker, 2005)'
_computing_data_collection       'SMART 5.054 (Bruker, 2003)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL 5.1, XP (Sheldrick, 1994)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      90(2)
_diffrn_detector_area_resol_mean 8.3
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker SMART 1000'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0510
_diffrn_reflns_av_sigmaI/netI    0.0301
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            28060
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.50
_diffrn_reflns_theta_min         1.48
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.471
_exptl_absorpt_correction_T_max  0.976
_exptl_absorpt_correction_T_min  0.895
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Twinabs (Sheldrick, 2003)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.791
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             810
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.968
_refine_diff_density_min         -0.752
_refine_diff_density_rms         0.081
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.046
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     534
_refine_ls_number_reflns         7924
_refine_ls_number_restraints     56
_refine_ls_restrained_S_all      1.085
_refine_ls_R_factor_all          0.0435
_refine_ls_R_factor_gt           0.0364
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0546P)²+1.3001P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0954
_refine_ls_wR_factor_ref         0.0997
_reflns_number_gt                6957
_reflns_number_total             7924
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            ic050426ksi20050322_093623.cif
_cod_data_source_block           mn1731
_cod_original_formula_sum        'H82 Al8 O68 S5'
_cod_database_code               4309215
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Al1 Al 0.23062(8) 0.34768(6) 0.49502(5) 0.00790(14) Uani 1 1 d . . .
Al2 Al 0.57938(8) 0.48101(6) 0.59608(5) 0.00817(14) Uani 1 1 d . . .
Al3 Al 0.41898(8) 0.19162(6) 0.62107(5) 0.00854(14) Uani 1 1 d . . .
Al4 Al 0.09703(8) 0.27315(6) 0.24585(5) 0.00950(14) Uani 1 1 d . . .
O1 O 0.43256(19) 0.38680(14) 0.46381(11) 0.0084(3) Uani 1 1 d D . .
H1 H 0.448(4) 0.334(2) 0.430(2) 0.019(8) Uiso 1 1 d D . .
O2 O 0.37705(18) 0.44951(15) 0.61629(11) 0.0088(3) Uani 1 1 d D . .
H2 H 0.360(4) 0.507(2) 0.638(2) 0.018(8) Uiso 1 1 d D . .
O3 O 0.23770(19) 0.48478(15) 0.44734(11) 0.0088(3) Uani 1 1 d D . .
H3 H 0.223(4) 0.543(2) 0.474(2) 0.024(8) Uiso 1 1 d D . .
O4 O 0.58015(19) 0.33992(14) 0.62996(12) 0.0098(3) Uani 1 1 d D . .
H4 H 0.672(3) 0.346(3) 0.658(2) 0.022(8) Uiso 1 1 d D . .
O5 O 0.25341(19) 0.21231(15) 0.53651(12) 0.0095(3) Uani 1 1 d D . .
H5 H 0.187(3) 0.147(2) 0.502(2) 0.025(9) Uiso 1 1 d D . .
O6 O 0.29524(19) 0.40621(15) 0.28501(12) 0.0102(3) Uani 1 1 d D . .
H6 H 0.328(4) 0.429(3) 0.2402(18) 0.020(8) Uiso 1 1 d D . .
O7 O 0.10766(19) 0.24926(15) 0.36826(11) 0.0098(3) Uani 1 1 d D . .
H7 H 0.080(4) 0.1751(18) 0.365(3) 0.030(9) Uiso 1 1 d D . .
O8 O 0.04892(19) 0.32840(15) 0.54008(12) 0.0109(3) Uani 1 1 d D . .
H8A H 0.045(4) 0.286(3) 0.579(2) 0.031(9) Uiso 1 1 d D . .
H8B H -0.045(3) 0.309(3) 0.507(2) 0.038 Uiso 1 1 d D . .
O9 O 0.5704(2) 0.15021(16) 0.70527(13) 0.0122(3) Uani 1 1 d D . .
H9A H 0.591(4) 0.158(3) 0.7643(13) 0.023(8) Uiso 1 1 d D . .
H9B H 0.633(4) 0.125(3) 0.686(2) 0.032(9) Uiso 1 1 d D . .
O10 O 0.2627(2) 0.03028(15) 0.60859(12) 0.0118(3) Uani 1 1 d D . .
H10A H 0.287(3) -0.018(2) 0.6355(19) 0.012(7) Uiso 1 1 d D . .
H10B H 0.167(3) 0.020(3) 0.608(2) 0.030(9) Uiso 1 1 d D . .
O11 O 0.4745(2) 0.11413(16) 0.51725(12) 0.0119(3) Uani 1 1 d D . .
H11A H 0.542(3) 0.158(3) 0.496(2) 0.032(9) Uiso 1 1 d D . .
H11B H 0.407(3) 0.059(3) 0.472(2) 0.048(12) Uiso 1 1 d D . .
O12 O 0.3698(2) 0.25434(15) 0.73319(12) 0.0115(3) Uani 1 1 d D . .
H12A H 0.277(2) 0.247(3) 0.727(2) 0.026(9) Uiso 1 1 d D . .
H12B H 0.429(3) 0.3263(19) 0.769(2) 0.027(9) Uiso 1 1 d D . .
O13 O 0.0695(2) 0.28084(17) 0.11462(13) 0.0159(4) Uani 1 1 d D . .
H13A H 0.045(4) 0.334(2) 0.095(2) 0.031(9) Uiso 1 1 d D . .
H13B H 0.092(5) 0.242(3) 0.073(2) 0.065(14) Uiso 1 1 d D . .
O14 O -0.11152(19) 0.13399(16) 0.19868(12) 0.0119(3) Uani 1 1 d D . .
H14A H -0.182(3) 0.130(3) 0.2273(19) 0.028(9) Uiso 1 1 d D . .
H14B H -0.162(4) 0.108(3) 0.1393(13) 0.039(10) Uiso 1 1 d D . .
O15 O -0.0180(2) 0.37635(16) 0.25540(13) 0.0134(3) Uani 1 1 d D . .
H15A H -0.100(3) 0.360(3) 0.274(3) 0.041(10) Uiso 1 1 d D . .
H15B H 0.027(4) 0.4532(17) 0.270(3) 0.037(10) Uiso 1 1 d D . .
O16 O 0.1921(2) 0.15821(16) 0.21383(12) 0.0124(3) Uani 1 1 d D . .
H16A H 0.288(2) 0.181(3) 0.247(2) 0.031(9) Uiso 1 1 d D . .
H16B H 0.147(3) 0.0856(18) 0.214(2) 0.023(8) Uiso 1 1 d D . .
O1W O 0.1052(2) 0.61809(17) 0.26802(14) 0.0175(4) Uani 1 1 d D . .
H1C H 0.095(4) 0.607(3) 0.2094(14) 0.025(9) Uiso 1 1 d D . .
H1D H 0.078(5) 0.675(3) 0.283(3) 0.066(14) Uiso 1 1 d D . .
O2W O -0.2575(3) 0.0317(3) 0.00587(19) 0.0464(6) Uani 1 1 d D . .
H2C H -0.305(10) -0.031(6) 0.027(6) 0.19(4) Uiso 1 1 d D . .
H2D H -0.328(8) 0.011(8) -0.051(3) 0.21(4) Uiso 1 1 d D . .
O3W O 0.5677(3) 0.4808(2) 0.84644(15) 0.0280(5) Uani 1 1 d D . .
H3D H 0.513(4) 0.521(3) 0.855(3) 0.046(12) Uiso 1 1 d D . .
H3C H 0.631(5) 0.492(4) 0.900(2) 0.082(17) Uiso 1 1 d D . .
O4W O 0.6517(3) 0.1843(3) 0.89663(17) 0.0551(8) Uani 1 1 d D . .
H4C H 0.7689 0.2749 0.9146 0.066 Uiso 0.50 1 d PD A 1
H4D H 0.6168 0.2002 0.9489 0.066 Uiso 0.50 1 d PD B 1
H4E H 0.7385 0.2592 0.9430 0.066 Uiso 0.50 1 d PD C 2
H4F H 0.6587 0.1214 0.9139 0.066 Uiso 0.50 1 d PD D 2
O5W O -0.4292(4) -0.1988(3) 0.0137(2) 0.0672(9) Uani 1 1 d D . .
H5D H -0.382(6) -0.244(4) 0.038(3) 0.081 Uiso 1 1 d D . .
H5C H -0.468(6) -0.179(4) 0.060(3) 0.081 Uiso 1 1 d D . .
O6W O 0.3754(4) 0.6037(3) 0.8636(2) 0.0579(8) Uani 1 1 d D . .
H6C H 0.335(7) 0.620(5) 0.811(2) 0.10(2) Uiso 1 1 d D . .
H6D H 0.443(7) 0.678(3) 0.899(4) 0.15(3) Uiso 1 1 d D . .
O7AW O 0.1541(5) 0.2323(3) -0.0499(3) 0.0247(11) Uani 0.536(6) 1 d P E 1
O7BW O 0.0310(6) 0.0904(5) -0.0254(3) 0.0382(15) Uani 0.464(6) 1 d P E 2
O8AW O 0.7447(13) 0.6037(11) 0.0545(8) 0.072(3) Uiso 0.33 1 d P F 1
O8BW O 0.7436(13) 0.5179(10) 0.0432(8) 0.058(3) Uiso 0.33 1 d P G 2
O8CW O 0.2113(13) 0.2832(10) -0.0941(8) 0.068(3) Uiso 0.33 1 d P H 3
S1 S 0.34778(7) 0.76090(5) 0.65183(4) 0.01091(12) Uani 1 1 d . . .
O17 O 0.3266(2) 0.86757(15) 0.70342(12) 0.0137(3) Uani 1 1 d . . .
O18 O 0.2768(2) 0.65286(17) 0.68691(15) 0.0219(4) Uani 1 1 d . . .
O19 O 0.2649(2) 0.73153(18) 0.54607(13) 0.0218(4) Uani 1 1 d . . .
O20 O 0.5200(2) 0.78877(16) 0.66266(12) 0.0142(3) Uani 1 1 d . . .
S2 S 0.92806(7) 0.08950(5) 0.67741(4) 0.00963(12) Uani 1 1 d . . .
O21 O 0.7633(2) 0.07547(16) 0.62697(13) 0.0159(4) Uani 1 1 d . . .
O22 O 0.9382(2) 0.07189(16) 0.77511(12) 0.0160(4) Uani 1 1 d . . .
O23 O 1.04519(19) 0.21609(15) 0.68715(12) 0.0121(3) Uani 1 1 d . . .
O24 O 0.96891(19) -0.00250(15) 0.61986(12) 0.0124(3) Uani 1 1 d . . .
S3A S -0.0240(4) 0.4962(3) 0.0031(2) 0.0075(6) Uiso 0.25 1 d P I -1
O25 O 0.0557(10) 0.5974(8) -0.0266(6) 0.0153(16) Uiso 0.25 1 d P I -1
O26 O 0.0421(15) 0.4873(10) 0.0934(8) 0.034(3) Uiso 0.25 1 d P I -1
O27 O -0.1653(13) 0.5044(9) 0.0161(6) 0.023(2) Uiso 0.25 1 d P I -1
O28 O -0.0751(10) 0.3761(8) -0.0687(6) 0.0199(17) Uiso 0.25 1 d P I -1
S3B S -0.0832(6) 0.4893(3) 0.0082(2) 0.0249(8) Uiso 0.25 1 d P J -2
O29 O -0.2074(16) 0.5227(10) 0.0232(8) 0.028(2) Uiso 0.25 1 d P J -2
O30 O 0.0768(16) 0.5793(14) 0.0816(10) 0.061(4) Uiso 0.25 1 d P J -2
O31 O -0.1182(16) 0.3688(12) 0.0195(9) 0.052(3) Uiso 0.25 1 d P J -2
O32 O -0.0915(11) 0.4956(8) -0.0932(6) 0.0152(19) Uiso 0.25 1 d P J -2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Al1 O7 86.98(8) . . ?
O3 Al1 O2 91.79(8) . . ?
O7 Al1 O2 172.67(8) . . ?
O3 Al1 O5 170.73(8) . . ?
O7 Al1 O5 92.46(8) . . ?
O2 Al1 O5 87.57(8) . . ?
O3 Al1 O8 97.62(8) . . ?
O7 Al1 O8 94.93(8) . . ?
O2 Al1 O8 92.40(8) . . ?
O5 Al1 O8 91.65(8) . . ?
O3 Al1 O1 80.21(7) . . ?
O7 Al1 O1 92.39(8) . . ?
O2 Al1 O1 80.27(7) . . ?
O5 Al1 O1 90.57(7) . . ?
O8 Al1 O1 172.25(8) . . ?
O3 Al1 Al2 38.77(5) . 2_666 ?
O7 Al1 Al2 86.15(6) . 2_666 ?
O2 Al1 Al2 88.37(6) . 2_666 ?
O5 Al1 Al2 131.95(6) . 2_666 ?
O8 Al1 Al2 136.36(6) . 2_666 ?
O1 Al1 Al2 41.67(5) . 2_666 ?
O3 Al1 Al2 88.04(6) . . ?
O7 Al1 Al2 134.17(6) . . ?
O2 Al1 Al2 38.51(5) . . ?
O5 Al1 Al2 85.70(6) . . ?
O8 Al1 Al2 130.87(6) . . ?
O1 Al1 Al2 41.95(5) . . ?
Al2 Al1 Al2 62.94(3) 2_666 . ?
O4 Al2 O6 98.17(8) . 2_666 ?
O4 Al2 O3 96.80(7) . 2_666 ?
O6 Al2 O3 90.53(8) 2_666 2_666 ?
O4 Al2 O2 90.00(7) . . ?
O6 Al2 O2 97.10(8) 2_666 . ?
O3 Al2 O2 168.97(8) 2_666 . ?
O4 Al2 O1 169.74(8) . 2_666 ?
O6 Al2 O1 91.54(8) 2_666 2_666 ?
O3 Al2 O1 79.70(7) 2_666 2_666 ?
O2 Al2 O1 92.10(7) . 2_666 ?
O4 Al2 O1 92.49(8) . . ?
O6 Al2 O1 168.80(8) 2_666 . ?
O3 Al2 O1 91.62(8) 2_666 . ?
O2 Al2 O1 79.38(7) . . ?
O1 Al2 O1 78.04(8) 2_666 . ?
O4 Al2 Al1 135.49(6) . 2_666 ?
O6 Al2 Al1 88.02(6) 2_666 2_666 ?
O3 Al2 Al1 38.84(5) 2_666 2_666 ?
O2 Al2 Al1 133.14(6) . 2_666 ?
O1 Al2 Al1 41.09(5) 2_666 2_666 ?
O1 Al2 Al1 86.78(6) . 2_666 ?
O4 Al2 Al1 88.61(6) . . ?
O6 Al2 Al1 135.50(6) 2_666 . ?
O3 Al2 Al1 132.48(6) 2_666 . ?
O2 Al2 Al1 38.68(5) . . ?
O1 Al2 Al1 86.77(5) 2_666 . ?
O1 Al2 Al1 40.89(5) . . ?
Al1 Al2 Al1 117.06(3) 2_666 . ?
O4 Al3 O5 96.03(8) . . ?
O4 Al3 O9 90.91(8) . . ?
O5 Al3 O9 172.98(8) . . ?
O4 Al3 O12 94.42(8) . . ?
O5 Al3 O12 93.26(8) . . ?
O9 Al3 O12 87.20(8) . . ?
O4 Al3 O11 89.35(8) . . ?
O5 Al3 O11 92.68(8) . . ?
O9 Al3 O11 86.36(8) . . ?
O12 Al3 O11 172.59(8) . . ?
O4 Al3 O10 175.05(8) . . ?
O5 Al3 O10 86.86(8) . . ?
O9 Al3 O10 86.15(8) . . ?
O12 Al3 O10 89.41(8) . . ?
O11 Al3 O10 86.50(8) . . ?
O6 Al4 O7 95.26(8) . . ?
O6 Al4 O15 92.67(8) . . ?
O7 Al4 O15 94.79(8) . . ?
O6 Al4 O13 90.32(8) . . ?
O7 Al4 O13 174.11(9) . . ?
O15 Al4 O13 86.81(8) . . ?
O6 Al4 O16 92.21(8) . . ?
O7 Al4 O16 92.94(8) . . ?
O15 Al4 O16 170.44(8) . . ?
O13 Al4 O16 84.95(8) . . ?
O6 Al4 O14 177.36(8) . . ?
O7 Al4 O14 87.37(8) . . ?
O15 Al4 O14 87.31(8) . . ?
O13 Al4 O14 87.04(8) . . ?
O16 Al4 O14 87.44(8) . . ?
Al1 O1 Al2 97.24(7) . 2_666 ?
Al1 O1 Al2 97.16(8) . . ?
Al2 O1 Al2 101.95(8) 2_666 . ?
Al1 O1 H1 120(2) . . ?
Al2 O1 H1 113(2) 2_666 . ?
Al2 O1 H1 123(2) . . ?
Al2 O2 Al1 102.81(8) . . ?
Al2 O2 H2 117(2) . . ?
Al1 O2 H2 116(2) . . ?
Al2 O3 Al1 102.38(8) 2_666 . ?
Al2 O3 H3 118(2) 2_666 . ?
Al1 O3 H3 125(2) . . ?
Al3 O4 Al2 133.57(10) . . ?
Al3 O4 H4 113(2) . . ?
Al2 O4 H4 113(2) . . ?
Al3 O5 Al1 134.41(10) . . ?
Al3 O5 H5 111(2) . . ?
Al1 O5 H5 113(2) . . ?
Al4 O6 Al2 132.61(10) . 2_666 ?
Al4 O6 H6 115(2) . . ?
Al2 O6 H6 111(2) 2_666 . ?
Al4 O7 Al1 134.20(10) . . ?
Al4 O7 H7 109(2) . . ?
Al1 O7 H7 112(2) . . ?
Al1 O8 H8A 111(2) . . ?
Al1 O8 H8B 127(2) . . ?
H8A O8 H8B 107(2) . . ?
Al3 O9 H9A 130(2) . . ?
Al3 O9 H9B 122(2) . . ?
H9A O9 H9B 108(2) . . ?
Al3 O10 H10A 121.9(19) . . ?
Al3 O10 H10B 120(2) . . ?
H10A O10 H10B 108(2) . . ?
Al3 O11 H11A 118(2) . . ?
Al3 O11 H11B 122(3) . . ?
H11A O11 H11B 108(3) . . ?
Al3 O12 H12A 118(2) . . ?
Al3 O12 H12B 120(2) . . ?
H12A O12 H12B 106(2) . . ?
Al4 O13 H13A 122(2) . . ?
Al4 O13 H13B 128(3) . . ?
H13A O13 H13B 110(3) . . ?
Al4 O14 H14A 121(2) . . ?
Al4 O14 H14B 120(2) . . ?
H14A O14 H14B 106(2) . . ?
Al4 O15 H15A 125(2) . . ?
Al4 O15 H15B 123(2) . . ?
H15A O15 H15B 106(2) . . ?
Al4 O16 H16A 114(2) . . ?
Al4 O16 H16B 120(2) . . ?
H16A O16 H16B 106(2) . . ?
H1C O1W H1D 106(3) . . ?
H2C O2W H2D 99(3) . . ?
H3D O3W H3C 107(3) . . ?
H4C O4W H4D 100.9 . . ?
H4C O4W H4E 29.2 . . ?
H4D O4W H4E 73.3 . . ?
H4C O4W H4F 120.0 . . ?
H4D O4W H4F 87.3 . . ?
H4E O4W H4F 108.8 . . ?
H5D O5W H5C 100(2) . . ?
H6C O6W H6D 101(3) . . ?
O18 S1 O20 110.48(10) . . ?
O18 S1 O17 110.24(11) . . ?
O20 S1 O17 111.25(10) . . ?
O18 S1 O19 108.97(12) . . ?
O20 S1 O19 106.50(10) . . ?
O17 S1 O19 109.31(10) . . ?
O22 S2 O21 110.47(11) . . ?
O22 S2 O24 110.14(10) . . ?
O21 S2 O24 108.93(10) . . ?
O22 S2 O23 108.42(10) . . ?
O21 S2 O23 109.27(10) . . ?
O24 S2 O23 109.61(10) . . ?
O26 S3A O25 119.3(6) . . ?
O26 S3A O27 98.5(6) . . ?
O25 S3A O27 107.8(5) . . ?
O26 S3A O28 109.0(6) . . ?
O25 S3A O28 113.9(5) . . ?
O27 S3A O28 106.5(5) . . ?
O29 S3B O31 107.8(7) . . ?
O29 S3B O32 102.6(6) . . ?
O31 S3B O32 113.1(6) . . ?
O29 S3B O30 109.6(7) . . ?
O31 S3B O30 110.3(8) . . ?
O32 S3B O30 113.0(7) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Al1 O3 1.8784(18) . ?
Al1 O7 1.8823(18) . ?
Al1 O2 1.8830(18) . ?
Al1 O5 1.8873(18) . ?
Al1 O8 1.8940(18) . ?
Al1 O1 1.9381(18) . ?
Al1 Al2 2.9252(11) 2_666 ?
Al1 Al2 2.9378(13) . ?
Al2 O4 1.8436(18) . ?
Al2 O6 1.8557(18) 2_666 ?
Al2 O3 1.8756(18) 2_666 ?
Al2 O2 1.8758(18) . ?
Al2 O1 1.9604(17) 2_666 ?
Al2 O1 1.9794(18) . ?
Al2 Al1 2.9252(11) 2_666 ?
Al3 O4 1.8423(18) . ?
Al3 O5 1.8600(17) . ?
Al3 O9 1.9092(18) . ?
Al3 O12 1.9095(18) . ?
Al3 O11 1.9141(18) . ?
Al3 O10 1.9200(19) . ?
Al4 O6 1.8503(18) . ?
Al4 O7 1.8545(18) . ?
Al4 O15 1.8980(18) . ?
Al4 O13 1.9098(19) . ?
Al4 O16 1.9239(18) . ?
Al4 O14 1.9395(19) . ?
O1 Al2 1.9604(17) 2_666 ?
O1 H1 0.812(18) . ?
O2 H2 0.794(18) . ?
O3 Al2 1.8756(18) 2_666 ?
O3 H3 0.812(18) . ?
O4 H4 0.825(18) . ?
O5 H5 0.800(18) . ?
O6 Al2 1.8557(18) 2_666 ?
O6 H6 0.831(18) . ?
O7 H7 0.824(18) . ?
O8 H8A 0.825(18) . ?
O8 H8B 0.822(18) . ?
O9 H9A 0.828(17) . ?
O9 H9B 0.819(17) . ?
O10 H10A 0.822(17) . ?
O10 H10B 0.845(17) . ?
O11 H11A 0.823(18) . ?
O11 H11B 0.805(18) . ?
O12 H12A 0.815(17) . ?
O12 H12B 0.844(18) . ?
O13 H13A 0.816(18) . ?
O13 H13B 0.823(19) . ?
O14 H14A 0.844(17) . ?
O14 H14B 0.838(18) . ?
O15 H15A 0.835(18) . ?
O15 H15B 0.834(18) . ?
O16 H16A 0.834(18) . ?
O16 H16B 0.824(17) . ?
O1W H1C 0.827(18) . ?
O1W H1D 0.817(19) . ?
O2W H2C 0.88(2) . ?
O2W H2D 0.87(2) . ?
O3W H3D 0.822(18) . ?
O3W H3C 0.829(19) . ?
O4W H4C 1.1758 . ?
O4W H4D 0.9135 . ?
O4W H4E 0.9828 . ?
O4W H4F 0.8533 . ?
O5W H5D 0.877(19) . ?
O5W H5C 0.873(19) . ?
O6W H6C 0.86(2) . ?
O6W H6D 0.88(2) . ?
S1 O18 1.4692(19) . ?
S1 O20 1.4718(18) . ?
S1 O17 1.4719(17) . ?
S1 O19 1.4910(19) . ?
S2 O22 1.4727(18) . ?
S2 O21 1.4731(18) . ?
S2 O24 1.4819(17) . ?
S2 O23 1.4879(18) . ?
S3A O26 1.369(11) . ?
S3A O25 1.381(9) . ?
S3A O27 1.394(12) . ?
S3A O28 1.486(9) . ?
S3B O29 1.388(14) . ?
S3B O31 1.415(13) . ?
S3B O32 1.491(9) . ?
S3B O30 1.518(14) . ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O16 H16A O20 0.834(18) 1.84(2) 2.656(2) 167(3) 2_666
O16 H16B O22 0.824(17) 1.828(18) 2.650(3) 175(3) 2_656
O1W H1C O30 0.827(18) 1.81(2) 2.637(14) 178(3) .
O1W H1C O26 0.827(18) 1.88(2) 2.596(11) 144(3) .
O1W H1C O32 0.827(18) 1.92(2) 2.653(9) 147(3) 2_565
O1W H1C O28 0.827(18) 2.08(2) 2.894(9) 166(3) 2_565
O1W H1D O23 0.817(19) 2.07(2) 2.866(2) 166(4) 2_666
O2W H2C O5W 0.88(2) 1.89(4) 2.705(5) 155(8) .
O2W H2D O4W 0.87(2) 2.38(8) 2.841(4) 113(7) 1_454
O3W H3D O6W 0.822(18) 1.878(19) 2.698(4) 175(4) .
O3W H3C O29 0.829(19) 1.95(2) 2.782(11) 176(5) 1_656
O3W H3C O8BW 0.829(19) 2.04(3) 2.857(11) 167(4) 1_556
O3W H3C O27 0.829(19) 2.18(2) 2.984(10) 164(4) 1_656
O4W H4E O28 0.98 1.87 2.631(9) 132.1 1_656
O4W H4E O25 0.98 2.02 2.987(9) 169.2 2_666
O4W H4E O31 0.98 1.54 2.522(14) 174.6 1_656
O4W H4F O2W 0.85 2.04 2.841(4) 155.2 1_656
O5W H5D O8CW 0.877(19) 1.86(3) 2.687(10) 157(5) 2
O5W H5D O7AW 0.877(19) 2.03(4) 2.660(5) 128(4) 2
O5W H5C O4W 0.873(19) 1.93(3) 2.715(4) 150(5) 2_556
O6W H6C O18 0.86(2) 1.93(2) 2.783(3) 170(6) .
O6W H6D O5W 0.88(2) 1.87(3) 2.691(5) 155(6) 1_666
